dL dZ2 dZ1dt dt dtdVF2 dZ 2 dZR10 R20dt dt dtdg0dt1 2if growing at 1-end (dZ 1 /dt>0)if not growing at 1-end (dZ 1 /dt

83. APPLICATION TO THE CASE OF GROWING FROM A NEARLY-SQUAREBARConsider an initially near-square bar (**of** uniform cross-section) **of** raw solid material, defined by its meanradius R i0 (e.g. R i0 =5 mm) and C i4 /R i0 =0.14 (the first coefficient **of** the Fourier cosine-expansion **of** asquare). If the figure-**of**-merit for "squareness" is defined by the ratio **of** the area **of** the inscribed square tothe area **of** the whole cross-section, a circle has a ratio **of** 2/=0.63, whereas with the fist harmonic it goesup to 0.95. To better grasp how much square the first harmonic gives, Fig. 3a shows the whole crosssection,but in Fig. 3b only two meridian cuts are shown: R =0 (i.e. maximum radii) and R =/4 (i.e.minimum radii). In the figures to follow, only these two radial pr**of**iles are used to visualise the 3D-shapein 2D plots.Fig. 3. Initial near-square solid bar in units **of** its mean radius R 1 : a) whole cross-section, b) only twomeridian cuts are shown: R(0)/R 1 (i.e. maximum radii, solid line) and R(/4)/R 1 (i.e. minimumradii, dash line). In the figures to follow, only these two radial pr**of**iles are used to visualise the3D-shape in 2D plots.Consider that a certain length L **of** this bar has been molten and assume that this is really the initial statefrom which **crystal** **growth** is to be simulated. The initial liquid interface is found from Eq. (22) andplotted in Fig. 4a for the cases **of** L/(2R 1 )=1 and two values **of** axial gravity, corresponding to B=0 andB=1; in this case, this large Bond value is still acceptable for the linear analysis **of** short liquid bridge (in arecent review [7] **of** the hydrostatics **of** liquid bridges with several loads, it can be seen that the maximumBond value for the present geometry is larger than 2). The 8% volume reduction upon melting for silicon**growth** has been accounted for and can be clearly appreciated in the figure. To see the effect **of** **non**-equalinitial supports, Fig. 4b has been computed to show the initial molten shape between a near-square and aperfect circular support **of** different sizes (R 10 /R 20 =0.8/1.2, L/(R 10 +R 20 )=1. Observe that, in any case, the**non**-**axisymmetric** effects only count near the **non**-circular ends, the liquid bridge tending to be**axisymmetric** in mid lengths.ab11RR / 0RR / 00011RR / 0RR / 0010ZR / 01010ZR / 01

9Fig. 4 Initial molten shape **of** slenderness =L/(2R 0 )=1 **of** the bar in Fig. 3 (the two extreme meridiansshown, for =0 solid, and for =/4 dashed) for the case **of** zero gravity (upper) and for an axialgravity corresponding to B=1 (lower), in units **of** the mean radius R 0 . In b, the effect **of** **non**-equalends (a square one with R 10 /R 0 =0.8 and a circular one with R 20 /R 0 =1.2 is shown.Now the simulated **crystal** **growth** process may be started by considering some pulling-heating lawequivalent to, say, a growing rate **of** dZ 1 /dt=10 5 m/s and constant molten length dZ 2 /dt=dZ 1 /dt (forconstant length evolution), and an adequate time step for the discrete **simulation** (say t=10 s), irrelevantfor the physics being simulated. Some results are presented in Fig. 5, simulating the **crystal** **growth** from anearly-square silicon rod with a molten **zone** **of** aspect ratio =0.5 (Fig. 5a), =1 (Fig. 5b), and =2 (Fig.5c), without external loads (B=0). It can be seen how the 11º **growth**-angle for silicon (Fig. 2) tends toneck the solid grown. Although the molten length, material properties and applied loads are kept constantin the three series, the more slender one (=2) shows unstable **growth** (neck breaking will follow). In anycase, both the grown solid and the molten **zone** tend to be **axisymmetric**, with the **non**-axisymmetrylimited to the ends.Fig. 5. Simulated **crystal** **growth** from an initially near-square silicon bar **of** mean radius R 0 and aspectratio =0.5, 1 and 2, without external loads (B=0), where it can be seen how the 11º **growth**-angle(Fig. 2) tends to neck the solid grown.The maximum slenderness **of** the molten **zone** for stable **crystal** **growth** depends on the applied loads, andin Fig. 6 the stable limits in the case **of** a constant axial load (residual acceleration) is presented as afunction **of** the slenderness, for the initially near-square bar. The upper limit **of** stability in Fig. 6corresponds to the molten bridge necking near the melting front (with fat **crystal** growing), and the lowerlimit to the molten bridge necking near the solidification front (with narrowing **crystal** **growth**).

10Fig. 6. Limiting axial loads (measured by the Bond number, B) for stable **crystal** **growth** from an initialliquid bridge obtained by **zone**-melting in a near-square silicon bar **of** mean radius R 0 , in the case**of** maintaining a constant molten length L. Growth shapes at a, b and c depicted in Fig. 7.To better appreciate the effect **of** an axial residual gravity on the **growth** and its stability, Fig. 7 has beenprepared by **simulation** **of** a **floating** **zone** process **of** constant molten length, =2, in an initially nearsquaresilicon bar, for the three loads corresponding to the three regions in Fig. 6: an axial load B=0.040in the middle **of** the stable region, and two unstable loads, B=0.010 and B=0.075, one at each side **of** thestability limits (check with Fig. 6).Fig. 7. Simulated **crystal** **growth** from an initially near-square silicon bar **of** mean radius R 0 , assuming afurnace control law such as to keep the molten length L constant all the time with =2,corresponding to the three cases marked in Fig. 6: axial loads B=+0.010 (a), B=+0.040 (b) andB=+0.075 (c), the middle one being the only stable **growth**.As said before, although most **of** the results here presented refer to an initial prismatic silicon bar with anear-square cross-section, the procedure here developed allows for any geometry **of** the end supports:unequal seed and feed sides, even eccentric, with the only bounds **of** the linear analysis based on thecylindrical geometry, that is for radial departures much smaller than the mean radius.CONCLUSIONSThe objective **of** this paper was to simulate the growing **of** **crystal**s **of** **non**-circular cross-section by the**floating** **zone** technique and analyse the sequence **of** shapes and their stability. This has been done byusing the hydrostatic liquid-bridge model (without any internal motions), shown in the literature to berepresentative **of** the mechanical behaviour in the real process.The **simulation** has been achieved by a mathematical model valid for shapes not too far from that **of** acylindrical molten **zone**. As an example, it has been applied to an initially near-square silicon bar, with aninitial departure from the mean cylinder **of** 14% to best approach a square cross-section, expecting anuncertainty in the results **of** the order **of** a few percent.As a general result, it has been found that there is a strong tendency for the liquid interface to get circular,and subsequently for the grown solid to get a circular cross-section, even if the initial rod is not **of** circularcross-section.

11Detailed results have been found for the maximum molten length allowing a stable **growth** (withoutnecking and bridge rupture) as a function **of** the residual axial gravity (measured by the Bond number).The algorithm developed could be directly applied to simulate the **growth** with different geometries anddifferent **growth** laws, within the linearised mathematical model.As a follow-on, a more closed-form analysis might be pursued, for instance to develop an analyticalexpression for the limits **of** stable **growth** as a function **of** the geometry and the loads, or a more appliednumerical **simulation** **of** the **non**-linear aspects (geometries far from the cylinder, large shapedeformations, and so on).ACKNOWLEDGEMENTSThis work has been supported by the Spanish Ministerio de Ciencia y Tecnología (MCYT).REFERENCES[1] Lan, C.W., Kou, S.: "Shortened **floating** **zone** **crystal** **growth** **under** normal gravity". J. CrystalGrowth 119, 281,291 (1992).[2] Cröll, A., Kaiser, T., Schweizer, M., Danilewsky, A.N., Lauer, S., Tegetmeier, A., and Benz, K.W.:"Floating-**zone** and **floating**-solution-**zone** **growth** **of** GaSb **under** microgravity". J. Crystal Growth191, 365, 376 (1998).[3] Martínez, I., Cröll, A.: "Liquid bridges and **floating** **zone**s". ESA SP-333, 135, 142 (1992).[4] Martínez, I., Eyer, A.: "Liquid bridge analysis **of** silicon **crystal** **growth** experiments **under**microgravity". J. Crystal Growth 75, 535, 544 (1986).[5] Boucher, E.A., Evans, M.J.B.: "A liquid-bridge model for the flat-**zone** processing **of** materials". J.Chem. Soc. Faraday Trans. I. 81, 2787, 2796 (1985).[6] Martínez, I., Perales, J.M.: "Mechanical behaviour **of** liquid bridges in microgravity in Physics **of**Fluids in Microgravity". in "Physics **of** Fluids in Microgravity", R. Monti (Ed.), Taylor & Francis,pp. 21-45, (2001).[7] Meseguer, J., Perales, J.M., Martínez, I., Bezdenejnykh, N.A., Sanz, A.: "Hydrostatic Instabilities inFloating Zone Crystal Growth Process". Current Topics in Crystal Growth Research 5, 27, 42(1999).[8] Rossolenko, S.N., Zhdanov, A.V.: "Equilibrium shapes **of** liquid menisci subjected to gravity forceand surface tension". J. Crystal Growth 104, 8, 13 (1990).[9] Pet'kov, I.S., Red'kin, B.S.: "Calculation **of** the stationary cross-section form **of** **non****axisymmetric**al**crystal**s growing from the melt". J. Crystal Growth 131, 598, 606 (1993).[10] Tatarchenko, V.A., Uspenski, V.S., Tatarchenko, E.V., Nobot, I.Ph., Duffar, T., Roux, B.:"Theoretical model **of** **crystal** **growth** shaping process". J. Crystal Growth 180, 615, 626 (1997).[11] Hamidi, M., Rodot, H.: "Experimental determination **of** the **growth** angle: application to silicon".Revue de Physique Appliquée 18, 75, 80 (1983).[12] Martínez, I., Sanz, A., Perales, J.M., Meseguer, J.: "Freezing **of** a Long Liquid Column on theTexus-18 Sounding Rocket Flight". ESA Journal 12, 483, 489 (1988).[13] Bezdenejnykh, N.A., Meseguer, J..: "On the use **of** liquid bridges as accelerometers". MicrogravitySci. Technol. 9, 62, 69 (1996).[14] Perales, J.M., Meseguer, J., Martinez, I.: "Minimum Volume **of** Axisymmetric Liquid Bridgesbetween Unequal Disks in an Axial Microgravity Field". J. Crystal Growth 110, 855, 861 (1991).[15] Martinez, I, Meseguer, J., Perales, J.M.: "Analytical Modelling **of** Floating Zone Crystal Growth".Adv. Space Res. Vol. 29, No. 4, pp. 569-574 (2002).